LMucko/crystallography-open-database huggingface dataset:
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 550 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010683
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 550 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.88292
_cell_length_b                   10.6447
_cell_length_c                   6.21066
_cell_formula_units_Z            4
_cell_volume                     322.813
_database_code_amcsd             0006661
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    4.174
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010683
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 600 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010684
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 600 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.88544
_cell_length_b                   10.6499
_cell_length_c                   6.21456
_cell_formula_units_Z            4
_cell_volume                     323.340
_database_code_amcsd             0006662
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    4.167
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010684
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 650 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010685
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 650 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.88766
_cell_length_b                   10.6543
_cell_length_c                   6.21842
_cell_formula_units_Z            4
_cell_volume                     323.822
_database_code_amcsd             0006663
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    4.161
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010685
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 700 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010686
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 700 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.89032
_cell_length_b                   10.6595
_cell_length_c                   6.22274
_cell_formula_units_Z            4
_cell_volume                     324.381
_database_code_amcsd             0006664
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    4.154
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010686
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 750 degree C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010687
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 750 degree C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.89292
_cell_length_b                   10.6653
_cell_length_c                   6.2270
_cell_formula_units_Z            4
_cell_volume                     324.953
_database_code_amcsd             0006665
_diffrn_ambient_temperature      1023.15
_exptl_crystal_density_diffrn    4.147
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010687
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 800 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010688
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 800 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.89570
_cell_length_b                   10.6711
_cell_length_c                   6.2309
_cell_formula_units_Z            4
_cell_volume                     325.518
_database_code_amcsd             0006666
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    4.140
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010688
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 850 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010689
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 850 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.89828
_cell_length_b                   10.6766
_cell_length_c                   6.2354
_cell_formula_units_Z            4
_cell_volume                     326.093
_database_code_amcsd             0006667
_diffrn_ambient_temperature      1123.15
_exptl_crystal_density_diffrn    4.132
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010689
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 900 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010690
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 900 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.9010
_cell_length_b                   10.6834
_cell_length_c                   6.2399
_cell_formula_units_Z            4
_cell_volume                     326.717
_database_code_amcsd             0006668
_diffrn_ambient_temperature      1173.15
_exptl_crystal_density_diffrn    4.124
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010690
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 950 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010691
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 950 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.9041
_cell_length_b                   10.6899
_cell_length_c                   6.2441
_cell_formula_units_Z            4
_cell_volume                     327.343
_database_code_amcsd             0006669
_diffrn_ambient_temperature      1223.15
_exptl_crystal_density_diffrn    4.116
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010691
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 1000 C
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010692
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 1000 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.9067
_cell_length_b                   10.6964
_cell_length_c                   6.2491
_cell_formula_units_Z            4
_cell_volume                     327.978
_database_code_amcsd             0006670
_diffrn_ambient_temperature      1273.15
_exptl_crystal_density_diffrn    4.108
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010692
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 800 C, Data collected on cooling
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010693
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 800 C, Data collected on cooling
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.8957
_cell_length_b                   10.6710
_cell_length_c                   6.2316
_cell_formula_units_Z            4
_cell_volume                     325.551
_database_code_amcsd             0006671
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    4.139
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010693
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 600 C, Data collected on cooling
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010694
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 600 C, Data collected on cooling
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.8850
_cell_length_b                   10.6490
_cell_length_c                   6.2141
_cell_formula_units_Z            4
_cell_volume                     323.260
_database_code_amcsd             0006672
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    4.168
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010694
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 550 C, Data collected on cooling
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010695
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 550 C, Data collected on cooling
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.8824
_cell_length_b                   10.6432
_cell_length_c                   6.2103
_cell_formula_units_Z            4
_cell_volume                     322.714
_database_code_amcsd             0006673
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    4.175
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010695
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 500 C, Data collected on cooling
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010696
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 500 C, Data collected on cooling
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.8798
_cell_length_b                   10.6376
_cell_length_c                   6.2060
_cell_formula_units_Z            4
_cell_volume                     322.149
_database_code_amcsd             0006674
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    4.183
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010696
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 450 C, Data collected on cooling
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010697
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 450 C, Data collected on cooling
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.8776
_cell_length_b                   10.6325
_cell_length_c                   6.2019
_cell_formula_units_Z            4
_cell_volume                     321.637
_database_code_amcsd             0006675
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    4.189
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010697
_amcsd_formula_title             FeMnSiO4
High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4 olivines: an in situ neutron diffraction study Sample: T = 400 C, Data collected on cooling
Redfern, S. A. T.; Henderson, C. M. B.; Knight, K. S.; Wood, B. J.; European Journal of Mineralogy 9 (1997) 287–300; doi:

data_9010698
_publ_section_title
;
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 400 C, Data collected on cooling
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              287
_journal_page_last               300
_journal_volume                  9
_journal_year                    1997
_chemical_formula_structural     FeMnSiO4
_chemical_formula_sum            'Fe Mn O4 Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.8754
_cell_length_b                   10.6260
_cell_length_c                   6.1980
_cell_formula_units_Z            4
_cell_volume                     321.094
_database_code_amcsd             0006676
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    4.197
_cod_original_formula_sum        '(Fe Mn) Si O4'
_cod_database_code               9010698
_amcsd_formula_title             FeMnSiO4